#------------------------------------------------------------------------------
#$Date: 2024-01-06 09:58:57 +0200 (Sat, 06 Jan 2024) $
#$Revision: 288793 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/24/77/7247774.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7247774
loop_
_publ_author_name
'Jones, Isabelle M.'
'Turner, Gemma F.'
'Pitts, Kari'
'Powell, Rees'
'Riboldi-Tunnicliffe, Alan'
'Williamson, Rachel'
'Boer, Stephanie'
'Allen, Lauren'
'Moggach, Stephen A.'
_publ_section_title
;
 High-pressure induced guest-mediated gate opening behaviour of the
 Co-based framework ZIF-67
;
_journal_issue                   47
_journal_name_full               CrystEngComm
_journal_page_first              6533
_journal_page_last               6538
_journal_paper_doi               10.1039/D3CE00979C
_journal_volume                  25
_journal_year                    2023
_chemical_absolute_configuration ad
_chemical_formula_moiety         'C8 H10 Co N4, 1.5[C2H5OH]'
_chemical_formula_sum            'C11 H19 Co N4 O1.5'
_chemical_formula_weight         290.23
_chemical_name_common            ZIF-67
_space_group_crystal_system      cubic
_space_group_IT_number           217
_space_group_name_Hall           'I -4 2 3'
_space_group_name_H-M_alt        'I -4 3 m'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     dual
_audit_creation_date             2023-10-02
_audit_creation_method
;
Olex2 1.5
(compiled 2023.08.24 svn.re1ec1418 for OlexSys, GUI svn.r6817)
;
_audit_update_record
;
2023-10-04 deposited with the CCDC.	2023-11-21 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            12
_cell_length_a                   17.1155(2)
_cell_length_b                   17.1155(2)
_cell_length_c                   17.1155(2)
_cell_measurement_reflns_used    983
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      18.6070
_cell_measurement_theta_min      1.6850
_cell_volume                     5013.82(10)
_computing_cell_refinement       'CrysAlisPro 1.171.42.58a (Rigaku OD, 2022)'
_computing_data_collection       'CrysAlisPro 1.171.42.58a (Rigaku OD, 2022)'
_computing_data_reduction        'CrysAlisPro 1.171.42.58a (Rigaku OD, 2022)'
_computing_molecular_graphics    'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2018/3 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXT  (Sheldrick, 2015)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector                 'Hybrid Pixel Array Detector'
_diffrn_detector_area_resol_mean 13.3333
_diffrn_measured_fraction_theta_full 0.937
_diffrn_measured_fraction_theta_max 0.933
_diffrn_measurement_details
;
List of Runs (angles in degrees, time in seconds):

  # Type    Start    End  Width  tₑₓₚ   ω     θ     κ     φ   Frames
#--------------------------------------------------------------------------
  1  φ    -31.60  35.00   0.10    0.10   0.00   0.00   0.00    --   666
;
_diffrn_measurement_device       'abstract diffractometer'
_diffrn_measurement_device_type
'dectris-CrysAlisPro-abstract goniometer imported dectris images'
_diffrn_measurement_method       'φ scans'
_diffrn_orient_matrix_type
'CrysAlisPro convention (1999,Acta A55,543-557)'
_diffrn_orient_matrix_UB_11      -0.0270075000
_diffrn_orient_matrix_UB_12      -0.0053143000
_diffrn_orient_matrix_UB_13      -0.0309013000
_diffrn_orient_matrix_UB_21      0.0048838000
_diffrn_orient_matrix_UB_22      -0.0410839000
_diffrn_orient_matrix_UB_23      0.0028426000
_diffrn_orient_matrix_UB_31      -0.0310869000
_diffrn_orient_matrix_UB_32      -0.0018131000
_diffrn_orient_matrix_UB_33      0.0274033000
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0494
_diffrn_reflns_av_unetI/netI     0.0532
_diffrn_reflns_Laue_measured_fraction_full 0.937
_diffrn_reflns_Laue_measured_fraction_max 0.933
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       9
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_number            1212
_diffrn_reflns_point_group_measured_fraction_full 0.897
_diffrn_reflns_point_group_measured_fraction_max 0.895
_diffrn_reflns_theta_full        18.600
_diffrn_reflns_theta_max         18.600
_diffrn_reflns_theta_min         1.683
_diffrn_source                   Synchrotron
_diffrn_source_type              'AS beamline MX1'
_exptl_absorpt_coefficient_mu    1.023
_exptl_absorpt_correction_T_max  0.7443
_exptl_absorpt_correction_T_min  0.4357
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
SADABS-2016/2 (Bruker,2016/2) was used for absorption correction.
wR2(int) was 0.1140 before and 0.0939 after correction.
The Ratio of minimum to maximum transmission is 0.5854.
The λ/2 correction factor is Not present.
;
_exptl_crystal_colour            'bluish violet'
_exptl_crystal_colour_modifier   bluish
_exptl_crystal_colour_primary    violet
_exptl_crystal_density_diffrn    1.153
_exptl_crystal_description       block
_exptl_crystal_F_000             1824
_exptl_crystal_size_max          0.15
_exptl_crystal_size_mid          0.1
_exptl_crystal_size_min          0.1
_platon_squeeze_details
;
TITL zif67_w2_70s_0051_a.res in I-43m
CELL   17.1155   17.1155   17.1155     90.00     90.00     90.00
SPGR I-43m
# Solvent Accessible Volume =      2531
# Electrons Found in S.A.V. =       456
# Note: Atoms in Void are Labelled as Cxxx and Qxxx for all Others
C101 0.357 0.638 0.362 !       1.04 eA-3
C102 0.622 0.371 0.488 !       0.66 eA-3
C103 0.122 0.871 0.988 !       0.66 eA-3
C104 0.122 0.988 0.871 !       0.66 eA-3
C105 0.685 0.690 0.482 !       0.65 eA-3
C106 0.403 0.408 0.543 !       0.61 eA-3
C107 0.575 0.583 0.340 !       0.61 eA-3
C108 0.080 0.080 0.080 !       0.61 eA-3
C109 0.334 0.334 0.334 !       0.56 eA-3
C110 0.467 0.467 0.467 !       0.54 eA-3
C111 0.640 0.702 0.437 !       0.51 eA-3
C112 0.197 0.072 0.204 !       0.50 eA-3
;
_refine_diff_density_max         0.091
_refine_diff_density_min         -0.128
_refine_diff_density_rms         0.023
_refine_ls_abs_structure_details
;
 Flack x determined using 124 quotients [(I+)-(I-)]/[(I+)+(I-)]
 (Parsons, Flack and Wagner, Acta Cryst. B69 (2013) 249-259).
;
_refine_ls_abs_structure_Flack   0.16(4)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.136
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     24
_refine_ls_number_reflns         350
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.137
_refine_ls_R_factor_all          0.0317
_refine_ls_R_factor_gt           0.0301
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0313P)²+1.2167P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0809
_refine_ls_wR_factor_ref         0.0816
_reflns_Friedel_coverage         0.683
_reflns_Friedel_fraction_full    0.844
_reflns_Friedel_fraction_max     0.845
_reflns_number_gt                329
_reflns_number_total             350
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            d3ce00979c2.cif
_cod_data_source_block           zif67_w2_70s_0051
_cod_depositor_comments
'Adding full bibliography for 7247762--7247779.cif.'
_cod_original_cell_volume        5013.82(18)
_cod_original_formula_sum        'C11 H19 Co N4 O1.50'
_cod_database_code               7247774
_shelx_shelxl_version_number     2018/3
_chemical_oxdiff_formula         'C10 H20 Co N4 O2'
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_max   0.905
_shelx_estimated_absorpt_t_min   0.862
_diffrn_orient_matrix_axis[1]    matrixX
_diffrn_orient_matrix_axis[2]    matrixY
_diffrn_orient_matrix_axis[3]    matrixZ
_olex2_refinement_description
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H) groups
 At 1.5 times of:
  All C(H,H,H) groups
2. Restrained planarity
 C3, N1, C2, C1
 with sigma of 0.1
3. Uiso/Uaniso restraints and constraints
Uanis(C3) = Uanis(N1) = Uanis(C2)
4. Others
 Fixed Sof: H1A(0.5) H1B(0.5) H1C(0.5)
5.a Aromatic/amide H refined with riding coordinates:
 C3(H3)
5.b Idealised Me refined as rotating group:
 C1(H1A,H1B,H1C)
;
_platon_squeeze_special_details
;
A solvent mask was calculated and 458 electrons were 
found in a volume of 2507Å³ in 1 void per unit cell. 
This is consistent with the presence of 
18[C2H5OH] per Unit Cell 
which account for 468 electrons 
per unit cell.
;
_platon_squeeze_void_probe_radius 1.20
_olex2_submission_special_instructions 'No special instructions were received'
_oxdiff_exptl_absorpt_empirical_details
;
Empirical correction (ABSPACK) includes:
- Absorption correction using spherical harmonics
- Frame scaling
;
_oxdiff_exptl_absorpt_empirical_full_max 4.715
_oxdiff_exptl_absorpt_empirical_full_min 0.336
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, z'
'-x, y, -z'
'x, -y, -z'
'z, x, y'
'z, -x, -y'
'-z, -x, y'
'-z, x, -y'
'y, z, x'
'-y, z, -x'
'y, -z, -x'
'-y, -z, x'
'y, x, z'
'-y, -x, z'
'y, -x, -z'
'-y, x, -z'
'x, z, y'
'-x, z, -y'
'-x, -z, y'
'x, -z, -y'
'z, y, x'
'z, -y, -x'
'-z, y, -x'
'-z, -y, x'
'x+1/2, y+1/2, z+1/2'
'-x+1/2, -y+1/2, z+1/2'
'-x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z+1/2'
'z+1/2, x+1/2, y+1/2'
'z+1/2, -x+1/2, -y+1/2'
'-z+1/2, -x+1/2, y+1/2'
'-z+1/2, x+1/2, -y+1/2'
'y+1/2, z+1/2, x+1/2'
'-y+1/2, z+1/2, -x+1/2'
'y+1/2, -z+1/2, -x+1/2'
'-y+1/2, -z+1/2, x+1/2'
'y+1/2, x+1/2, z+1/2'
'-y+1/2, -x+1/2, z+1/2'
'y+1/2, -x+1/2, -z+1/2'
'-y+1/2, x+1/2, -z+1/2'
'x+1/2, z+1/2, y+1/2'
'-x+1/2, z+1/2, -y+1/2'
'-x+1/2, -z+1/2, y+1/2'
'x+1/2, -z+1/2, -y+1/2'
'z+1/2, y+1/2, x+1/2'
'z+1/2, -y+1/2, -x+1/2'
'-z+1/2, y+1/2, -x+1/2'
'-z+1/2, -y+1/2, x+1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Co1 Co 0.000000 -0.500000 -0.250000 0.0938(8) Uani 1 4 d S T P . .
N1 N 0.0321(3) -0.5899(4) -0.3168(3) 0.0970(15) Uani 1 1 d . . . . .
C2 C -0.0081(8) -0.6227(3) -0.3773(3) 0.0970(15) Uani 1 2 d S T P . .
C1 C -0.0854(6) -0.5938(6) -0.4062(6) 0.118(4) Uani 1 2 d S T P . .
H1A H -0.126697 -0.592517 -0.358283 0.177 Uiso 0.5 1 calc R U P A -1
H1B H -0.106780 -0.632490 -0.451477 0.177 Uiso 0.5 1 calc R U P A -1
H1C H -0.078592 -0.535464 -0.429771 0.177 Uiso 0.5 1 calc R U P A -1
C3 C 0.1002(4) -0.6304(4) -0.3124(4) 0.0970(15) Uani 1 1 d . . . . .
H3 H 0.146516 -0.619815 -0.271217 0.116 Uiso 1 1 calc R U . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_axis.id
_axis.type
_axis.equipment
_axis.parity
_axis.depends_on
_axis.zero
_axis.vector[1]
_axis.vector[2]
_axis.vector[3]
source . source . . . 1.00000000 0.00000000 0.00000000
omega rotation goniometer -1 . 0.00000000 0.00000000 0.00000000 1.00000000
kappa rotation goniometer -1 omega 0.00000000 -0.76604444 0.00000000 0.64278761
phi rotation goniometer -1 kappa . 0.00000000 0.00000000 1.00000000
theta rotation goniometer -1 . 0.00000000 0.00000000 0.00000000 1.00000000
matrixX general general . phi . 1.00000000 0.00000000 0.00000000
matrixY general general . phi . 0.00000000 1.00000000 0.00000000
matrixZ general general . phi . 0.00000000 0.00000000 1.00000000
dacX translation general . phi . 0.00000000 1.00000000 0.00000000
dacY translation general . phi . -1.00000000 0.00000000 0.00000000
dacZ translation general . phi . 0.00000000 0.00000000 1.00000000
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
N1 Co1 N1 109.19(16) . 40_444 ?
N1 Co1 N1 109.20(16) 40_444 2_545 ?
N1 Co1 N1 110.0(3) . 2_545 ?
N1 Co1 N1 109.20(16) . 39_544 ?
N1 Co1 N1 110.0(3) 40_444 39_544 ?
N1 Co1 N1 109.20(16) 39_544 2_545 ?
C2 N1 Co1 127.8(5) . . ?
C3 N1 Co1 126.8(4) . . ?
C3 N1 C2 105.4(7) . . ?
N1 C2 N1 111.7(9) 20_544 . ?
N1 C2 C1 124.1(5) . . ?
N1 C2 C1 124.1(5) 20_544 . ?
C2 C1 H1A 109.5 . . ?
C2 C1 H1B 109.5 . . ?
C2 C1 H1C 109.5 . . ?
H1A C1 H1B 109.5 . . ?
H1A C1 H1C 109.5 . . ?
H1B C1 H1C 109.5 . . ?
N1 C3 C3 108.8(4) . 20_544 ?
N1 C3 H3 125.6 . . ?
C3 C3 H3 125.6 20_544 . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Co1 N1 1.994(5) . ?
Co1 N1 1.994(5) 39_544 ?
Co1 N1 1.994(5) 2_545 ?
Co1 N1 1.994(5) 40_444 ?
N1 C2 1.365(8) . ?
N1 C3 1.357(7) . ?
C2 C1 1.496(14) . ?
C1 H1A 1.0831 . ?
C1 H1B 1.0831 . ?
C1 H1C 1.0831 . ?
C3 C3 1.384(13) 20_544 ?
C3 H3 1.0770 . ?
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
Co1 N1 C2 N1 179.6(3) . . . 20_544 ?
Co1 N1 C2 C1 2.0(14) . . . . ?
Co1 N1 C3 C3 -179.3(4) . . . 20_544 ?
C2 N1 C3 C3 -0.5(6) . . . 20_544 ?
C3 N1 C2 N1 0.9(11) . . . 20_544 ?
C3 N1 C2 C1 -176.7(10) . . . . ?
loop_
_platon_squeeze_void_nr
_platon_squeeze_void_average_x
_platon_squeeze_void_average_y
_platon_squeeze_void_average_z
_platon_squeeze_void_volume
_platon_squeeze_void_count_electrons
_platon_squeeze_void_content
1 -0.013 -0.006 -0.004 2507 458 ' '
loop_
_platon_missing_refln_index_h
_platon_missing_refln_index_k
_platon_missing_refln_index_l
_platon_missing_refln_theta
0 0 2 2.380
0 3 7 9.098
